10 hours ago - ... thermites based on Co(0) aerogels is the efficiency (100%) by which the ... (1) That definition has been expanded to include materials whose ...
Ernesto Carmona Feted as an Icon of Organometallic Chemistry ... ACS Editors' Choice: Air Quality in Puerto Rico in the Aftermath of Hurricane Maria â and ...
31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53 ...... residual liquids were collected for the photograph under ultraviolet and ...
Apr 12, 2019 - The maximum CD grafting content on the CNF-based aerogel was 113 mg gâ1, providing bright blue fluorescence under ultraviolet radiation ...
3 hours ago - Taking the innovation of an organic solvent-free route and avoiding the toxic crosslinking reagents or fluorescent ... View: PDF | PDF w/ Links.
Apr 12, 2019 - (2) Originated from their intrinsic microstructure, aerogels commonly exhibit exceptional properties, for instance, an extremely high porosity ...
May 8, 2017 - Polyisocyanate based aerogels combine ultralow thermal conductivities with better mechanical properties than silica aerogel, but these properties critically depend on the nature of ..... This implies that the more chemical cross-links t
May 8, 2017 - Polyisocyanate based aerogels combine ultralow thermal conductivities with better mechanical properties than silica aerogel, but these properties critically depend on the nature of the gelation solvent, perhaps more so than on any other
May 8, 2017 - Superinsulating Polyisocyanate Based Aerogels: A Targeted Search for the Optimum Solvent System ... Phone: + 41 58 765 4983.
May 8, 2017 - insulation,1,2 catalysis,3â5 oil-spill cleanup,6 CO2 capture,7â10 etc. Aerogels can ... sizes are small compared to the mean free path length of air (70 .... Spectral data of a PURâPIR aerogel (sample #12 from. Table 3) .... in a
A Cobalt Sunrise: Thermites Based on LiClO4‑Filled Co(0) Aerogels Prepared from Polymer-Cross-Linked Cobaltia Xerogel Powders Parwani M. Rewatkar, Rushi U. Soni, Chariklia Sotiriou-Leventis,* and Nicholas Leventis* Department of Chemistry, Missouri University of Science and Technology, Rolla, Missouri 65409, United States
Downloaded by ALBRIGHT COLG at 18:27:53:863 on June 11, 2019 from https://pubs.acs.org/doi/10.1021/acsami.9b04734.
S Supporting Information *
ABSTRACT: A new route to metallic aerogels that bypasses the use of supercritical ﬂuids and handling fragile wet-gel and aerogel precursors is exempliﬁed by the carbothermal synthesis of monolithic Co(0) aerogels from compressed cobaltia xerogel powders coated conformally (cross-linked) at the primary particle level with a carbonizable polyurea. Residual carbon is removed, and carbon-free samples are obtained by high-temperature treatment of as-prepared Co(0) aerogels under a ﬂowing stream of H2O/H2 that prevents oxidation of the Co(0) network. The durability of Co(0) aerogels is demonstrated under harsh processing conditions in their application as thermites. For this, Co(0) aerogel discs are inﬁltrated with LiClO4 from a melt and are ignited at about 1100 °C with an electric resistor. As Co(0) “burns” to CoO, temperature exceeds 1500 °C, and the heat released (552 ± 2 kcal mol−1) is near to both the theoretical value (−58.47 kcal mol−1) and that from well-known pressed-pellet iron/perchlorate thermites (−66.6 kJ mol−1). The advantage of nanostructured thermites based on Co(0) aerogels is the eﬃciency (100%) by which the metal is consumed during its reaction with LiClO4 ﬁlling the pores. KEYWORDS: cobalt, aerogel, xerogel, carbothermal, thermite
long diﬀusion time needed in order for cross-linking reagents and solvents to inﬁltrate the interior of large monolithic wetgels and thus reach, react, and latch on the skeletal nanoparticles throughput. That issue is further compounded by the drying process of wet-gels to aerogels that typically involves converting the pore-ﬁlling solvent into a supercritical ﬂuid (SCF) that is vented oﬀ like a gas. Alternatively, we have demonstrated recently that large monolithic SiC and Si3N4 aerogels can be prepared by pyrolysis of compressed compacts of X-silica xerogel powders obtained from suspensions of sol− gel particles, which in turn were obtained by disrupting gelation of silica sols with vigorous stirring.18 That method does not involve molding and handling fragile wet-gels and/or aerogels, bypassing the use of SCF for drying wet-gels into aerogels, or the need for long drying times for converting wetgels into xerogels. That is, the short time/distance that reagents and solvents need to diﬀuse over in order to access the interior of the wet-gel grains of the suspension cuts down the cross-linking process from days to minutes. High porosity was created when the cross-linking polymer reacted away during carbothermal reduction of silica toward the carbide or the nitride. Here, that methodology is extended to large-sized monolithic metallic Co(0) aerogels for which a route through monolithic aerogel precursors could not have even been practical, as reportedly only a few selected cobaltia sols can gel and they do so with great diﬃculty (gelation time ∼10 days).19 Received: March 16, 2019 Accepted: May 29, 2019
0.43 M) with aqueous HCl. Figure 1 shows that the spectrum of the [Co(H2O)6]Cl2 in DMF was practically the same as that
The durability of the newly prepared Co(0) aerogels was probed under extreme processing conditions: the porous space of Co(0) aerogels was ﬁlled almost completely with molten LiClO4; the resulting composites did not shrink, remained monolithic, and were demonstrated as thermites20 analogous to pressed Fe(0)/KClO4 pellets that are used in thermal batteries.21,22
2. RESULTS AND DISCUSSION The overall process to Co(0) aerogels and their operation as thermites is summarized in Scheme 1. Synthetic procedures are Scheme 1. Synthesis of Co(0) Aerogels and Their Implementation as Thermites
Figure 1. Spectrophotometric titration of a [Co(H2O)6](NO3)2 solution in DMF (0.43 M, red line) with HCl (black dashed lines, fractions denote the HCl/[Co(H2O)6](NO3)2 mol/mol ratio). As the concentration of HCl increases, the intensity of the absorption at 523 nm decreases (red arrow pointing down) and the intensity at 675 nm increases. The blue line shows the spectrum of [Co(H2O)6]Cl2 in DMF at the same concentration (0.43 M). Concentrations of the cobalt complexes were equal to those used in the sol. Spectra were taken from undiluted solutions using a sample holder with an optical path of 0.09 mm.
of the nitrate salt plus 4 equiv of HCl, suggesting that gelation of the hexahydrate salt with epichlorohydrin (Scheme 2, reaction 2) was convoluted with reaction 1, the equilibrium of which lies to the left. Reasonably, reaction 1 is expected to be also involved at the surface of the CoOx particles resulting from reaction 3. Indeed, prior TEM work has shown that cobaltia nanoparticles do form in our sol.13 Furthermore, the thermogravimetric (TGA) proﬁle of CoOx (Figure 2a) shows two mass loss events in the 200−400 °C range (pointed at by blue arrows); reasoning by analogy to Co(OH)2 and Co2(OH)3Cl,19,28 the ﬁrst mass loss, which is observed at around 220 °C, is assigned to dehydroxylation of −OH-capped cobaltia nanoparticles, while the second one, at around 300 °C, involves the loss of chlorine from −Cl-capped particles. The presence of a signiﬁcant amount of surface −Cl caps suggests a reduced aptitude for cobaltia nanoparticles to develop interparticle Co−O−Co bridges, which are a prerequisite for gelation. Notwithstanding the reasons that prevent large-scale gelation, as outlined in the Introduction, this work bypasses the need to make monolithic cobaltia aerogels (or xerogels) toward metallic Co(0) aerogels. The multidisperse irregular grains of the precipitate from reaction 3 (Figure 3a, left) had an internal nanostructure typical of oxide sol−gel materials (xerogel or aerogel) (Figure 3a, right). The skeletal density ρs of the CoOx xerogel powder was 3.137 ± 0.003 g cm−3, and the BET surface area σ was 62.4 m2 g−1. The primary particle diameter was about 31 nm [=6/(ρs × σ)], and agreed with the minimum particle size in SEM (Figure 3a, right) and previous TEM results.13 In TGA (Figure 2a), the CoOx xerogel powder lost about 3% of its mass by 200 °C (attributed to solvent) and another 25% by
detailed in the Experimental Section. Comprehensive materials characterization data are compiled in Table S1. The sections below discuss the rationale, chemical transformations, and characterization data of the various intermediates along with processing. 2.1. Preparation of Cobaltia (CoOx) Powder. Cobaltia (CoOx) suspensions were produced from DMF sols via the reaction of [Co(H2O)6]Cl2 with a proton acceptor (epichlorohydrin).24−26 For characterization purposes, part of the suspension was centrifuged and the precipitate was washed and dried under vacuum. Importantly, the [Co(H2O)6]Cl2 salt is pink, but its DMF solutions were blue suggesting that octahedral [Co(H2O)6]2+ was in equilibrium with tetrahedral [CoCl4]2− (Scheme 2, reaction 1).27 The position of that equilibrium was evaluated by titrating a DMF solution of [Co(H2O)6](NO3)2 (at the same concentration as in the sol: Scheme 2. Chemical Processes during Preparation of Cobaltia (CoOx)
68.49% w/w and was identiﬁed as CoO (Figure 2b). Thus, CoOx contained about 54% w/w Co. 2.2. Cross-Linking of CoOx with a Carbonizable Polyurea: Preparation of X-CoOx. Cross-linking was carried out by adding an aromatic triisocyanate (TIPM, see reaction 4) to CoOx suspensions and heating (Scheme 1). The size of
the grains in the new material (X-CoOx) remained unchanged; under high magniﬁcation, skeletal particles were still visible, albeit a massive uptake of polymer. While both CoOx and XCoOx powders were attracted by laboratory magnets, treating X-CoOx powder with aqueous HCl (12 M) yielded a residue that was not magnetic. TGA under O2 showed that CoOx was removed almost completely; the residue at 1000 °C was just 3.3% w/w (Figure 2a). Solid-state 13C NMR (Figure S1) showed that the residue was chemically identical to polyurea (PUA) obtained via the reaction of TIPM with water (reaction 4).26 The skeletal density of the X-CoOx powder dropped to ρs = 1.734 ± 0.003 g cm−3, and the BET surface area also decreased to σ = 36.2 m2 g−1. Lower ρs and σ values increased the apparent particle diameter to about 96 nm. Concurrently, the speciﬁc pore volume in the 1.7−300 nm range V1.7−300nm (Table S1) decreased to 0.11 cm3 g−1 (from 0.35 cm3 g−1 in CoOx), consistent with PUA coating the primary CoOx particles and ﬁlling the space in between them. At 1000 °C under O2, X-CoOx gave a TGA residue of 30.3% w/w (CoO, see Figure 2a,b); therefore, it was concluded that X-CoOx contained 23.8% Co. Considering the skeletal density of X-CoOx as the weighted average of the ρs values of CoOx (3.137 ± 0.003 g cm−3) and of TIPM-derived polyurea (1.24 g cm−3),29 the PUA-to-CoOx mass ratio in X-CoOx was calculated equal to 0.74:0.26. Given that, (a) at 800 °C under Ar, the char yield of TIPM-derived polyurea is 56% w/w29 and (b) that char consists of 81% w/w C (the balance being N/O in a ∼1:1 atomic ratio),29 the carbon yield of X-CoOx at 800 °C was expected to be about 33.6% w/w. Since X-CoOx contains 23.8% w/w Co (see the last paragraph above), the expected C/Co mol/mol ratio from carbonization of X-CoOx was equal to 7.0. Given that, at 800 °C, CoOx yields Co3O4 (Figure 2b), the reduction process at 800 °C requires 2 mol of C per mol of Co3O4 for conversion to Co(0) and CO2.10 Therefore, it was concluded that the expected C/Co ratio from X-CoOx was suﬃcient for reduction of the latter to Co(0). 2.3. Compaction of X-CoOx Powder to Discs. Using diﬀerent dies, X-CoOx powder was compressed under 10000 psi into diﬀerent size discs (see the Experimental Section). The compaction pressure has not been optimized; the value of 10000 psi was selected because it is within the typical range used for compressing pellets for infrared spectroscopy; therefore, it is easily accessible in most laboratories, rendering reproduction of this work rather straightforward. Compaction did not alter the oxidation state of cobalt. In XPS, the Co 2p spectra of CoOx powder, compressed CoOx powder (at 10000 psi), and compressed X-CoOx (at 10000 psi) discs were identical (Figure 4), consisting of two major peaks corresponding to the Co 2p1/2 and Co 2p3/2 energy levels
Figure 2. (a) TGA under O2 at 5 °C min−1 of CoOx (blue line), XCoOx (red line), and HCl-treated X-CoOx (dashed black line). Blue arrows point at the two decomposition steps of CoOx in the 200−400 °C range (see text). (b) Referring to panel (a) (blue line): XRD of the residue from TGA under O2 collected at 800 and 1000 °C, as indicated.
Figure 3. SEM images of (a) CoOx powder (left: grains; right: interior of the grains), (b) X-CoOx compressed disc at two magniﬁcations, (c) as-prepared Co(0)/C (before carbon removal), (d) Co(0)-800 (i.e., Co(0) aerogel after carbon removal with H2O/ H2 at 800 °C), (e) Co(0)-900 (i.e., Co(0) aerogel after carbon removal with H2O/H2 at 900 °C), and (f) monolithic CoO after ignition of LiClO4-loaded Co(0)-900 aerogels and washing with water.
400 °C, attributed to dehydroxylation and loss of Cl as discussed above. By 900 °C, TGA under O2 (Figure 2a) yielded a 73.20% w/w residue that was identiﬁed with XRD as Co3O4 (Figure 2b); by 1000 °C, the residue was reduced to C
CoOx were squeezed together, were both evident in the SEM image (Figure 3b). 2.4. Carbothermal Reduction of X-CoOx Compact Discs and Removal of Residual Carbon. Reduction of XCoOx compacts was carried out at 800 °C under ﬂowing Ar (Scheme 1). Discs came out black and remained monolithic. Their bulk density was 2.14 ± 0.02 g cm−3. XRD showed only one crystalline phase (α-Co) (Figure 5), but the skeletal
Figure 5. Powder XRD spectra of samples as shown. Numerical extensions denote the temperature of the last processing step (see text). Figure 4. High-resolution Co 2p XPS spectra of CoOx powder (top), a CoOx compressed pellet (middle), and of a X-CoOx compressed disc (bottom).
density (3.80 ± 0.09 g cm−3) was much lower than the density of metallic Co (8.90 g cm−3). SEM showed bright metallic protrusions embedded in amorphous matter (Figure 3c). CHN analysis yielded 41.55 ± 0.2% C w/w. Despite shrinkage (31.56 ± 0.19% in linear dimensions, see Table S1), the porosity (44% v/v) was more than twice the porosity of the X-CoOx compressed discs (19.9% v/v). In TGA under O2, the product lost 31.31% of its mass up to 900 °C and an additional 4.49% by 1000 °C (Figure 6). The ﬁrst mass loss was attributed to unreacted carbon and conversion of Co(0) to Co3O4, while the second mass loss was due to conversion of Co3O4 to CoO (as discussed in conjunction with Figure 2). By either value, the atomic ratio of unreacted C-to-Co(0) was 4.83, which is in reasonable agreement with the after-pyrolysis expected atomic ratio of C/Co (7.0) and the 1:2 mol/mol stoichiometry of the reduction of Co3O4 to Co(0) and CO2 (see above).10 A demanding application of Co(0) aerogels is as thermites for thermal batteries.20,21 Because of the conﬁned space in the latter devices, combustion of residual carbon would cause an explosion. A second cause of explosion is the rapid heating and expansion of the pore ﬁlling air.11,32 This type of explosion is facilitated by weakening of the metallic network under oxidative carbon removal (e.g., with O2 at 600 °C).32 Thus, our approach here was ﬁrst to remove carbon under conditions that would provide an overwhelmingly reducing environment around Co(0) and second to ﬁll the pores with the oxidant (LiClO4) almost completely. Carbon was removed with water vapor using H2 as the carrier gas at two diﬀerent temperatures, namely, 800 and 900 °C. (It is noted that if the carrier gas for the water vapor is Ar, while all other conditions remain the same, Co(0) is oxidized
(at around 797 and 781 eV, respectively), with a spin-energy separation of about 15.8 eV and two higher-energy satellite features at around 802 and 785 eV, all characteristic of Co(II) species.30,31 Just like the X-CoOx powders, compressed XCoOx discs were attracted by laboratory magnets. Gram magnetic susceptibilities were measured, and the values were reduced to magnetic susceptibilities per gram of Co. Thus, the susceptibilities per gram of Co of the CoOx powder and of the [Co(H2O)6]Cl2 complex were close to one another (193.35 and 179.94, respectively; theoretical value for the hexahydrated complex: 164.76, all in cgs units ×10−6); similarly, the susceptibilities per gram of Co of the X-CoOx powder and of the X-CoOx compressed discs were higher yet close to one another (229.70 and 233.07, respectively, again in cgs units ×10−6), suggesting a direct chemical interaction (bonding) between Co(II) and the polymer, as expected from crosslinking14 and that interaction was not altered under 10000 psi. The skeletal density of the X-CoOx compacts (1.673 ± 0.009 g cm−3) was practically unchanged from that of the loose X-CoOx powder (see Section 2.2). Based on the ρs value and the bulk density of the compact discs (1.340 ± 0.007 g cm−3), their porosity was calculated at 19.9% v/v. The values of V1.7−300nm and σ (0.0561 cm3 g−1 and 19.5 m2 g−1, respectively) were about half relative to those of the X-CoOx powders. The majority of the speciﬁc pore volume (62%) was assigned to pores >300 nm in diameter. Fusion of the X-CoOx aggregates and macroporosity, presumably created when grains of XD
reagents (as pointed out in the Introduction, xerogels react more eﬃciently than corresponding aerogels13), the low surface area of Co(0)-900 was of low concern as long as the porous space was large enough to accommodate the amount of oxidizer (LiClO4) needed for complete consumption of Co(0). Indeed, from skeletal and bulk density data (3.16 ± 0.07 g cm−3), open porosity was suﬃciently high (62% v/v), and it should be able to accommodate the amount of LiClO4 needed for complete combustion of the Co(0) in the aerogel discs. 2.5. Filling the Porous Space of Co(0) Aerogels with LiClO4 and Ignition. Co(0) aerogels were ﬁlled with LiClO4 via capillary action from a melt in a sublimation apparatus under vacuum at 270 °C. CAUTION: This is a highly energetic system, and all safety rules must be obeyed at all times (see the Experimental Section). The Co(0)-LiClO4 pellets did not shrink relative to the Co(0) aerogels (Scheme 1 and Table S1). α-Co remained the only Co(0) phase. Based on bulk and skeletal density data (3.86 ± 0.20 and 4.122 ± 0.056 g cm−3, respectively), the porosity of the LiClO4-loaded Co(0) pellets was reduced to 6.4% v/v (from 62% v/v before inﬁltration with LiClO4). Based either on those skeletal density data or the mass gain of the Co(0)-LiClO4 pellets, the amount of LiClO4 was 1.01 ± 0.01 mol/mol relative to the amount required for complete combustion via reaction 5.
Figure 6. TGA (at 5 °C min−1) of samples and conditions as follows. Black line: under O2 of an as-prepared Co(0)/C-800 disc; blue line: under O2 of a carbon-free Co(0)-900 disc; red line: under N2 of a carbon-free C(0)-900 disc. Numerical extensions denote the temperature of the last processing step (see text).
completely to CoOby XRD, data not shown.) In SEM, the 800 °C samples had a more open structure than the 900 °C samples (compare Figure 3d,e). (For further comparison of the properties of the two materials, refer to Table S1.) For thermites, we opted to proceed with the 900 °C samples because smaller pores had the tendency to retain molten LiClO4 longer, thus minimizing its spillage, which may reduce the amount of oxidizer available for combustion of the Co(0) network. Post carbon-removal CHN analysis yielded 0.12 ± 0.02% w/w C, −0.03 ± 0.005% w/w H, and 0.02 ± 0.005% w/ w N. XRD showed only one crystalline phase (α-Co) over a ﬂat baseline (Figure 5). TGA under N2 of carbon-free Co(0) aerogels showed essentially a ﬂat proﬁle up to 1000 °C (Figure 6). TGA under O2 showed ﬁrst a 135.9% mass increase up to 922.2 °C (expected for Co(0)-to-Co3O4: 136.20% w/w) and a subsequent decrease to 127.3% (expected for Co(0)-to-CoO: 127.15%). (The chemical identity of the two residues at the two temperatures was conﬁrmed with XRDjust as in Figure 2b.) Macroscopically, Co(0) aerogels from the 900 °C treatment for carbon removal (referred to as Co(0)-900 samples) were silvery-gray and extremely sturdy with a Young’s modulus of 689 ± 10 MPa and ultimate compressive strength of 1035 ± 19 MPa at over 80% strain (see Figure S2). By comparison, the Young’s moduli of ceramic SiC and Si3N4 aerogels made by the same method described here (i.e., from xerogel powders) were much lower (37 and 59 MPa, respectively),18 and iron aerogels made from interpenetrating networks had to be annealed at 1200−1300 °C to reach the same density as the Co(0)-900 aerogels, yet their Young’s modulus was less than half (316 MPa).32 The distribution of open pores in the Co(0)-900 samples was centered at 11 μm (by Hg intrusion, see Figure S3). The skeletal density of the same samples was 8.2 ± 0.1 g cm−3 (versus 8.90 g cm−3 for pure Co(0)) indicating 7.45% v/ v closed porosity along the metallic framework. Consistent with SEM, the BET surface area was low (0.46 m2 g−1). However, given that intimate contact of solid-state reagents is as important, or even more so, as how ﬁnely divided are the
4Co(0) + LiClO4 → 4CoO + LiCl
For ignition, Nichrome wire was wrapped around the Co(0)-LiClO4 discs (Figure 7). Ignition started at one of the
Figure 7. Ignition (t = 0) and combustion of a LiClO4-inﬁltrated Co(0)-900 aerogel disc (21.8 diameter, 3.7 mm thick). The arrow shows the point of ignition. The temperature at the center of the disc at t = 4 s after ignition reached 1515 °C (see Movie S2).
contact points of the disc with the wire when the temperature of the latter was approximately 1100 °C (calculated as described in the Experimental Section). Once ignition started, the electric power to the wire was disconnected, and further combustion was self-sustained. A very bright glow spread rapidly throughout the disc. Quickly, that glow turned red and then ceased altogether. It took about 20 s from ignition to complete combustion (see Movies S1 and S2). Using an infrared pyrometer, the disc temperature reached 1515 °C. Discs shrunk slightly during combustion (Table S1) but kept their shape. After combustion, discs were washed with water and were dried. However, they remained monolithic (Scheme 1), and the only crystalline phase was CoO (Figure 5). Fused CoO particles were <100 nm in size (Figure 3f). The ρs value of the CoO network was 5.06 ± 0.03 g cm−3 (density of CoO = 6.44 g cm−3), pointing to 27% v/v closed porosity. The skeletal and the bulk density (2.686 ± 0.023 g cm−3) of the E
volume of the centrifuged paste, was added to the centrifuge tubes containing the CoOx slurry from the last ethyl acetate wash, the tubes were sealed tightly with their caps, and the suspension was heated in an oven at 65 °C for 24 h. The mixture was swirled frequently to redistribute the settled powder and increase the diﬀusion rate. At the end of the 24 h period, the tubes were allowed to cool to room temperature, they were centrifuged for 15 to 20 min, and the suspension was washed 5× with ethyl acetate as above. Always, the wash solvent was removed using centrifugation. Again, for all washes, the volume of solvent was 2× the volume of the paste at the bottom of the centrifuge tubes. After removing the solvent from the last ethyl acetate wash, the contents of the tubes were transferred with the aid of small portions of ethyl acetate and were combined in a roundbottom ﬂask. Ethyl acetate was removed, and the product was dried under reduced pressure at 80 °C into a dry, freely ﬂowing X-CoOx powder. 4.1.3. Preparation of Monolithic Co(0) Aerogels. Dry X-CoOx powder was compressed into discs using aluminum dies and a hydraulic press operated at 10000 psi. Two diﬀerent dies were used yielding two diﬀerent size discs (diameter/thickness, mm/mm): 41.9/ 7.6 and 13.0/3.9. Placement of the powder in the dies was carried out in small portions under continuous tapping to ensure even distribution and settling of the X-CoOx powder. Compressed discs were reduced at 800 °C for 5 h under ﬂowing high-purity Ar. At the end of the heating period, the furnace was allowed to cool down under ﬂowing Ar, pellets were removed, and it was found that they contained unreacted carbon. Those samples are referred to as Co(0)/ C-800, whereas the numerical extension indicates the temperature of their treatment. Unreacted carbon was removed with H2O-saturated H2. For this, the temperature of the tube furnace was raised to either 800 or 900 °C under ﬂowing Ar, the gas was switched to H2Osaturated H2, and the temperature was held at that point for 36 h. (Flowing H2 was saturated with water vapor by bubbling through water before it was directed to the furnace.) At the end of this period, the furnace was allowed to cool down under a continuous ﬂow of H2. The resulting samples are referred to as Co(0)-800 or as Co(0)-900 where the numerical extension indicates the temperature used for their preparation. 4.1.4. Preparation of LiClO4-Loaded Co(0)-900 Aerogels. Co(0)900 samples were degassed at 80 °C overnight under vacuum prior to perchlorate inﬁltration. The inﬁltration process was carried out in sublimation apparatus under vacuum at 270 °C (melting point of LiClO4 = 236 °C). The sublimation apparatus containing solid LiClO4 and a hanging Co(0) aerogel pellet at the bottom of the top lid was sealed and heated under vacuum to the intended temperature using a sand bath. The pellet was held in place with a magnetic rod placed inside the “cold” ﬁnger of the sublimation apparatus. After LiClO4 melted completely, the magnetic rod was pulled out of the cold ﬁnger, and the Co(0)-900 aerogel pellet dropped in the pool of molten LiClO4. In the beginning, the Co(0)-900 pellet ﬂoated on the liquid perchlorate, but eventually it sunk as it was ﬁlled with the liquid salt. The process took 15−20 min. At the end of this period, the pellet was removed from the molten salt, always under vacuum, with the help of a powerful Nd-Fe-B magnet from the outside. Subsequently, the apparatus was allowed to cool to room temperature, the vacuum was broken, and the perchlorate-inﬁltrated pellet was removed. The amount of perchlorate was determined gravimetrically. CAUTIONARY NOTE: With the understanding that one deals with a highly energetic system, all safety precautions must be obeyed during inf iltration: (a) face and body protection must be used; (b) the inf iltration vessel must be placed behind a Plexiglass shield inside a f ume hood; and (c) a Class D33 f ire extinguisher must be kept next to the f ume hood at all times. 4.2. Methods. 4.2.1. Pyrolytic Synthesis of Co(0). Pyrolytic conversion of X-CoOx compacts to pure metallic cobalt aerogels was carried out in a programmable MTI GSL1600X-80 tube furnace (outer and inner tubes both of 99.8% pure alumina; outer tube: 1022 mm × 82 mm × 70 mm; inner tube: 610 mm × 61.45 mm × 53.55 mm; length of the heating zone at the set temperature: 457 mm). The
CoO discs together gave an open porosity of 47% v/v. The sum of open and closed porosity (74% v/v) was near the sum of those values in the Co(0)-900 aerogels (70% v/v). Ignition of Co(0)-LiClO4 in a bomb calorimeter under highpurity Ar (1 bar, 23 °C) yielded again CoO as the only cobalt phase (identical XRD proﬁle as the one shown in Figure 5, top). The heat released (−55.17 ± 2.01 kcal per mol of Co(0) reacted) was close to both the theoretical value (−58.47 kcal mol−1 from reaction 5) and the heat released from the analogous combustion of Fe(0) to FeO (−66.6 kcal mol−1).32 Thus, LiClO4-ﬁlled Co(0) aerogels comprise a reasonable alternative to pressed-pellet iron/KClO4 thermites. One advantage of the nanostructured cobalt system over the pressed pellet technology is that Co(0) is consumed completely.
3. CONCLUSIONS Deconvolution of the synthesis of monolithic non-oxide aerogels from monolithic aerogel precursors has been extended to smeltable metals. Other possible candidates include Fe, Ni, Sn, and Cu. According to the new method, both metallic and ceramic aerogels can be prepared from X-xerogel powders, relying for porosity on the carbonizable cross-linking polymer reacting away. Using xerogel powders as precursors renders the whole process economical because it speeds up solvent exchanges and bypasses time-consuming SCF- or freeze-drying. In the present case of Co(0) aerogels, further streamlining was achieved by removing unreacted C with H2O/H2. Application of Co(0) aerogels in thermites was a point of departure in order to demonstrate durability at high temperatures, in melts, and in contact with strong oxidizers. It follows that less demanding environments as in liquiﬁed gases or electrolytic solutions will be tolerated easily. Applications of Co(0) aerogels in catalysis as porous electrodes and in magnetic separations are underway. 4. EXPERIMENTAL SECTION 4.1. Materials. All reagents and solvents were used as received. Epichlorohydrin (EPH) was purchased from Sigma Aldrich Chemical Co. Cobalt chloride hexahydrate (CoCl2·6H2O) and HPLC grade dimethylformamide (DMF) and ethyl acetate (EtOAc) were purchased from Fisher Scientiﬁc International, Inc. Tris(4-isocyanatophenylmethane) (TIPM) was donated by Covestro LLC (Pittsburg, PA) as a 27% w/w solution in dry EtOAc under the trade name Desmodur RE. Ultra-high-purity Ar (grade 5) and H2 (99.999% purity) gases were purchased from Ozarc Gas (Rolla, MO). 4.1.1. Preparation of CoOx Suspensions. CoCl2·6H2O (15.756 g, 0.06622 mol) was dissolved in DMF (100 mL) under vigorous stirring. Epichlorohydrin (55 mL, 0.632 mol) was added, and the blue solution was heated at 80 °C for 120 min. A suspension (CoOx) started forming in about 15−20 min. After the heating period, the mixture was allowed to cool down to room temperature, and stirring was continued for another 24 h. The CoOx suspension was transferred to centrifuge tubes (50 mL, Fischer Scientiﬁc), and the solvent was exchanged three times with ethyl acetate. All washes and solvent exchanges were carried out with centrifugation for 15−20 min at 2450 rpm. For each solvent exchange/wash step, the new solvent that was brought in was 2× the volume of the compacted slurry (paste) at the bottom of the centrifuge tubes. Before every new centrifugation step, the compacted CoOx slurry was resuspended with a glass rod. For characterization purposes, a portion of the slurry from the last wash was dried under reduced pressure at 80 °C into a dry, freely ﬂowing CoOx powder. 4.1.2. Preparation of Cross-Linked X-CoOx Powder. As-received Desmodur RE (i.e., a solution of TIPM in ethyl acetate), 1× the F
ACS Applied Materials & Interfaces rate of heating and cooling was always maintained at 2.5 °C min−1. All gas ﬂow rates were set at 325 mL min−1. 4.2.2. Ignition of LiClO4-Loaded Co(0)-900 Aerogel Pellets. For ignition in open air, Nichrome wire (0.65 mm in diameter) was wrapped around LiClO4-loaded Co(0)-900 pellets, and power was supplied to the wire with a Variac. The voltage across the wire (8.5 V) was measured with a multimeter, and the electric current ﬂowing through the wire (13.0 A) was measured using a Fluke i400 inductive current probe. Using the diameter of the wire, the current ﬂowing through it, and by consulting tables,34 the temperature at the point of ignition was about 1100 °C. That temperature was also conﬁrmed with an infrared thermometer. The whole setup was placed in a fume hood behind a Plexiglass shield. Videos were recorded with a Sony Handycam Model DCR-SR68 placed on a tripod. The temperature of the LiClO4-loaded Co(0)-900 pellets during thermite operation was monitored with an infrared thermometer (Model 0S3708) from Omega Engineering, Inc. focused at the center of the disc. The maximum temperature recorded was 1515 °C (Movie S2). 4.2.3. Physical Characterization. Bulk densities (ρb) were calculated from the weight and the physical dimensions of the samples. Skeletal densities (ρs) were determined with helium pycnometry using a Micromeritics AccuPyc II 1340 instrument. Samples for skeletal density measurements were outgassed for 24 h at 80 °C under vacuum before analysis. Percent porosities Π were determined from the ρb and ρs values via Π = 100 × (ρs − ρb)/ρs. 4.2.4. Thermogravimetric Analysis (TGA). TGA was conducted under N2 or O2 with a TA Instruments Model TGA Q50 thermogravimetric analyzer using a heating rate of 5 °C min−1. 4.2.5. Chemical Characterization. Diﬀerent methods were applied at diﬀerent stages of processing as follows. CHN elemental analysis was conducted with an Exeter Analytical Model CE440 elemental analyzer, calibrated with acetanilide. The combustion furnace was operated at 925 °C. The calibration standard and samples were run three times, and results are given as averages. The cross-linking polymer was identiﬁed as TIPM-derived polyurea with solid-state CPMAS 13C NMR on a Bruker Avance III 400 MHz spectrometer with a carbon frequency of 100 MHz, using a 7 mm Bruker MAS probe at a magic angle spinning rate of 5 kHz with broadband proton suppression, and CP total suppression of spinning sidebands (TOSS) pulse sequence. The TOSS pulse sequence was applied by using a series of four properly timed 180° pulses on the carbon channel at diﬀerent points of a cycle before the acquisition of the FID, after an initial excitation with a 90° pulse on the proton channel. The 90° excitation pulse on the proton and the 180° excitation pulse on carbon were set to 4.2 and 10 μs, respectively. The cross-polarization contact time and the relaxation delay were set at 2000 ms and 5 s, respectively. The number of scans was set at 2048. Spectra were referenced externally to glycine (carbonyl carbon at 176.03 ppm). Chemical shifts are reported versus TMS (0 ppm). For this, dry X-CoOx powder was treated for 30 min with aqueous HCl (12 M). At the end of the period, the suspension was washed several times with water and several times with acetone. The ﬁnal slurry was dried under vacuum at 80 °C overnight. X-CoOx powders were attracted by magnets; after removal of the CoOx component with HCl, they were not. The NMR spectrum of the residue was compared with the spectrum of polyurea obtained from the reaction of TIPM with water. Powder X-ray diﬀraction (XRD) analysis was performed with powders of the corresponding materials using a PANalytical X’Pert Pro multipurpose diﬀractometer (MPD) with Cu Kα radiation (λ = 1.54 Å) and a proportional counter detector equipped with a ﬂat graphite monochromator. X-ray photoelectron spectroscopic analysis (XPS) was carried out with a Kratos Axis 165 Photoelectron Spectroscopy System. Samples were mixed and ground together with Au powder (5% w/w) as internal reference. Samples were analyzed as powders. Each sample was placed on a piece of conductive carbon tape that was adhered to a stainless steel sample holder. Samples were introduced into the analysis chamber one at a time, and the chamber was evacuated at 10−8 torr or lower. No ion sputtering was performed on any of the
samples. An Al monochromatic source (150 W) was used for excitation. A charge neutralizer was used to reduce the eﬀects of diﬀerential or sample charging. The analysis area was 700 × 300 microns. Elemental quantiﬁcation calculations were based on broad survey results from single sweeps at higher sensitivity (pass energy = 80) and were carried out with the Kratos Axis Vision processing software taking into consideration the appropriate relative sensitivity factors for the particular XPS system. High-resolution elemental scans were carried out at a lower sensitivity (pass energy = 20) using multiple sweeps to improve the signal-to-noise ratios. Deconvolution of Co 2p spectra was performed with Gaussian function ﬁtting using the OriginPro 8.5.1 software package. UV−vis spectroscopy was carried out in DMF solutions of CoCl2· 6H2O, Co(NO3)2·6H2O, and Co(NO3)2·6H2O with varying concentrations of HCl using a Cary 5000 UV−vis Spectrophotometer Model G9825A. Absorbance was recorded from 270 to 800 nm. Samples were referenced against DMF. The salt concentration in each solution was 0.43 M, equal to the concentration of CoCl2·6H2O in the DMF sol used for making CoOx suspensions. Five diﬀerent solutions of Co(NO3)2·6H2O in DMF were prepared by varying the molar ratio of HCl/[Co(NO3)2·6H2O] as follows: 1:4, 1:2, 1:1, 2:1, and 4:1. Magnetic susceptibilities were measured with powders of the corresponding samples using a Johnson Matthey Model Mark I Magnetic Susceptibility Balance. A ﬁve-point calibration curve was constructed with CoCl2·6H2O, CuSO4·6H2O, K3[Fe(CN)6], CoO, and H2O. The mass magnetic susceptibility χg (in cgs units) was calculated using the following equation:35 χg = CL(R − Ro)/[1 × 109(m)], where C is the balance calibration constant, L is the sample height in centimeter, R is the reading from the digital display when the sample and the tube are in place in the instrument, Ro is the reading from the display when the empty sample tube is placed in the instrument, and m is the sample mass in gram. 4.2.6. Solid Framework Characterization. Scanning electron microscopy (SEM) was conducted with Au-coated samples on a Hitachi Model S-4700 ﬁeld-emission microscope. 4.2.7. Pore Structure Analysis. N2-sorption porosimetry at 77 K was conducted with a Micromeritics ASAP 2020 surface area and porosity analyzer. Samples for N2-sorption analysis were outgassed for 24 h at 80 °C under vacuum before analysis. The pore size distribution of the Co pellet was also probed with Hg-intrusion porosimetry using a Micromeritics AutoPore IV 9500 instrument. 4.2.8. Mechanical Characterization of Co(0) Aerogels. Quasistatic compression testing of Co(0)-900 aerogels at low strain rates (2.5 mm/mm) was conducted on an Instron 4469 Universal Testing Machine using a 50 kN load cell, following testing procedures and specimen length/diameter ratios in the spirit of ASTM D1621-04a (Standard Test Method for Compressive Properties of Rigid Cellular Plastics), as described before.16 The recorded force as a function of displacement (machine-compliance corrected) was converted into stress as a function of strain. 4.2.9. Calorimetry. The enthalpy of the reaction taking place in LiClO4-impregnated Co(0) was measured in a 200 mL bomb calorimeter (Parr Instrument Company, Model 1108 Oxygen Combustion Vessel and Model 1341 Plain Jacket Calorimeter). The heat capacity of the calorimeter was measured using benzoic acid as the standard. The sample was ignited with Nichrome fuse wire (0.65 mm in diameter, 10 cm in length) connected to the terminal socket on the apparatus head, which in turn was connected to the ignition unit (Variac). The experiment was carried out by heating the Nichrome wire with a supply of 13.0 A current for 15 s under an atmosphere of high-purity Ar. The heat released by the fuse was measured independently with the calorimeter and was taken into consideration in the calculations. After each experiment, the residue was collected and analyzed with XRD.
S Supporting Information *
The Supporting Information is available free of charge on the ACS Publications website at DOI: 10.1021/acsami.9b04734. G
Materials characterization data; solid-state 13C NMR; compression data; Hg porosimetry (PDF) Ignition of pellets to combustion (MPG) Ignition of pellets to combustion in sync with an infrared thermometer (MPG)
aldehyde Nanoparticle Networks to Porous Metals and Carbides. J. Mater. Chem. 2010, 20, 7456−7471. (14) Leventis, N. Three-Dimensional Core-Shell Superstructures: Mechanically Strong Aerogels. Acc. Chem. Res. 2007, 40, 874−884. (15) Leventis, N.; Sotiriou-Leventis, C.; Zhang, G.; Rawashdeh, A.M. M. Nanoengineering Strong Silica Aerogels. Nano Lett. 2002, 2, 957−960. (16) Leventis, N.; Sotiriou-Leventis, C.; Mulik, S.; Dass, A.; Schnobrich, J.; Hobbs, A.; Fabrizio, E. F.; Luo, H.; Churu, G.; Zhang, Y.; Lu, H. Polymer Nanoencapsulated Mesoporous Vanadia with Unusual Ductility at Cryogenic Temperatures. J. Mater. Chem. 2008, 18, 2475−2482. (17) Meador, M. A. B.; Capadona, L. A.; MacCorkle, L.; Papadopoulos, D. S.; Leventis, N. Structure-Property Relationships in Porous 3D Nanostructures as a Function of Preparation Conditions: Isocyanate Cross-Linked Silica Aerogels. Chem. Mater. 2007, 19, 2247−2260. (18) Rewatkar, P. M.; Taghvaee, T.; Saeed, A. M.; Donthula, S.; Mandal, C.; Chandrasekaran, N.; Leventis, T.; Shruthi, T. K.; Sotiriou-Leventis, C.; Leventis, N. Sturdy, Monolithic SiC and Si3N4 Aerogels from Compressed Polymer-Cross-Linked Silica Xerogel Powders. Chem. Mater. 2018, 30, 1635−1647. (19) Peterson, G. R.; Hung-Low, F.; Gumeci, C.; Bassett, W. P.; Korzeniewski, C.; Hope-Weeks, L. J. Preparation−Morphology− Performance Relationships in Cobalt Aerogels as Supercapacitors. ACS Appl. Mater. Interfaces 2014, 6, 1796−1803. (20) Overviews of Recent Research on Energetic Materials. In Advanced Series in Physical Chemistry; Shaw, R. W., Brill, T. B., Thompson, D. L., Eds.; World Scientiﬁc Publishing, Co.: London, U.K., 2005; Vol. 16. (21) Guidotti, R. A.; Masset, P. Thermally Activated (“Thermal”) Battery technology. J. Power Sources 2006, 161, 1443−1449. (22) Thermal batteries include an electrolytic salt that becomes an ionic conductor after melting through the heat provided by a thermite. Alternatively, the electrolytic salt can form an ionic conductor by dissolution; thus, the same concept has been extended to wet-condition indicators.23 (23) See for example: Leventis, N.; Galison, W. A. Apparatus for Detecting Moisture in Garments. U.S. Patent No. 5,796,345 1998. (24) Simpson, Randall L.; Gash, A. E.; Tillotson, T. M.; Satcher, J. H., Jr.; Poco, J. F.; Hrubesh, L. W.; Simpson, R. L. Use of Epoxides in the Sol−gel Synthesis of Porous Iron(III) Oxide Monoliths from Fe(III) Salts. Chem. Mater. 2001, 13, 999−1007. (25) Fears, T. M.; Sotiriou-Leventis, C.; Winiarz, J. G.; Leventis, N. Economical Synthesis of Vanadia Aerogels via Epoxide-Assisted Gelation of VOCl3. J. Sol-Gel Sci. Technol. 2016, 77, 244−256. (26) Leventis, N.; Vassilaras, P.; Fabrizio, E. F.; Dass, A. Polymer Nanoencapsulated Rare Earth Aerogels: Chemically Complex but Stoichiometrically Similar Core-Shell Superstructures with Skeletal Properties of Pure Compounds. J. Mater. Chem. 2007, 17, 1502− 1508. (27) Greenwood, N. N.; Earnshaw, A. Chemistry of the Elements; Butterworth-Heinemann: Woburn, MA 1998, p 1131. (28) García-Martínez, O.; Millán, P.; Rojas, R. M.; Torralvo, M. J. Cobalt Basic Salts as Inorganic Precursors of Cobalt Oxides and Cobalt Metal: Thermal behaviour Dependence on Experimental Conditions. J. Mater. Sci. 1988, 23, 1334−1350. (29) Leventis, N.; Sotiriou-Leventis, C.; Chandrasekaran, N.; Mulik, S.; Larimore, Z. J.; Lu, H.; Churu, G.; Mang, J. T. Multifunctional Polyurea Aerogels from Isocyanates and Water. A Structure-Property Case Study. Chem. Mater. 2010, 22, 6692−6710. (30) Cobalt: Transition Metal. https://xpssimpliﬁed.com/elements/ cobalt.php (Accessed 05-27-2019) (31) Xie, S.; Liu, Y.; Deng, J.; Yang, J.; Zhao, X.; Han, Z.; Zhang, K.; Dai, H. Insights into the Active Sites of Ordered Mesoporous Cobalt Oxide Catalysts for the Total Oxidation of o-xylene. J. Catal. 2017, 352, 282−292.
The authors declare no competing ﬁnancial interest.
ACKNOWLEDGMENTS This project was supported by ARO (W911NF-14-1-0369) and the NSF (1530603). We thank Covestro LLC for the generous supply of Desmodur RE (TIPM) and Dr. J. Watts for access to his infrared thermometer.
(1) Leventis, N.; Sadekar, A.; Chandrasekaran, N.; Sotiriou-Leventis, C. Click Synthesis of Monolithic Silicon Carbide Aerogels from Polyacrylonitrile-Coated 3D Silica Networks. Chem. Mater. 2010, 22, 2790−2803. (2) Vareda, J. P.; Lamy-Mendes, A.; Durães, L. A Reconsideration on the Definition of the Term Aerogel based on Current Drying Trends. Microporous Mesoporous Mater. 2018, 258, 211−216. (3) Du, A.; Zhou, B.; Zhang, Z.; Shen, J. A Special Material or a New State of Matter: A Review and Reconsideration of the Aerogel. Materials 2013, 6, 941−968. (4) Tappan, B. C.; Steiner, S. A., III; Luther, E. P. Nanoporous Metal Foams. Angew. Chem., Int. Ed. 2010, 49, 4544−4565. (5) Cai, B.; Dianat, A.; Hübner, R.; Liu, W.; Wen, D.; Benad, A.; Sonntag, L.; Gemming, T.; Cuniberti, G.; Eychmüller, A. Multimetallic Hierarchical Aerogels: Shape Engineering of the Building Blocks for Efficient Electrocatalysis. Adv. Mater. 2017, 29, 1605254. (6) Liu, W.; Herrmann, A.-K.; Bigall, N. C.; Rodriguez, P.; Wen, D.; Oezaslan, M.; Schmidt, T. J.; Gaponik, N.; Eychmüller, A. Noble Metal Aerogels−Synthesis, Characterization, and Application as Electrocatalysts. Acc. Chem. Res. 2015, 48, 154−162. (7) Wen, D.; Herrmann, A.-K.; Borchardt, L.; Simon, F.; Liu, W.; Kaskel, S.; Eychmüller, A. Controlling the Growth of Palladium Aerogels with High-Performance toward Bioelectrocatalytic Oxidation of Glucose. J. Am. Chem. Soc. 2014, 136, 2727−2730. (8) Wakayama, H.; Fukushima, Y. Porous Platinum Fibers Synthesized Using Supercritical Fluid. Chem. Commun. 1999, 391− 392. (9) Bozbag, S. E.; Sanli, D.; Erkey, C. Synthesis of Nanostructured Materials Using Supercritical CO2: Part II. Chemical Transformations. J. Mater. Sci. 2012, 47, 3469−3492. (10) Shen, Y. Carbothermal Synthesis of Metal-functionalized Nanostructures for Energy and Environmental Applications. J. Mater. Chem. A 2015, 3, 13114−13188. (11) Mahadik-Khanolkar, S.; Donthula, S.; Bang, A.; Wisner, C.; Sotiriou-Leventis, C.; Leventis, N. Polybenzoxazine Aerogels. 2. Interpenetrating Networks with Iron Oxide and the Carbothermal Synthesis of Highly Porous Monolithic Pure Iron(0) Aerogels as Energetic Materials. Chem. Mater. 2014, 26, 1318−1331. (12) Leventis, N.; Chandrasekaran, N.; Sotiriou-Leventis, C.; Mumtaz, A. Smelting in the Age of Nano: Iron Aerogels. J. Mater. Chem. 2009, 19, 63−65. (13) Leventis, N.; Chandrasekaran, N.; Sadekar, A. G.; Mulik, S.; Sotiriou-Leventis, C. The Effect of Compactness on the Carbothermal Conversion of Interpenetrating Metal Oxide / Resorcinol-FormH
ACS Applied Materials & Interfaces (32) Leventis, N.; Donthula, S.; Mandal, C.; Ding, M. S.; SotiriouLeventis, C. Explosive versus Thermite Behavior in Iron(0) Aerogels Infiltrated with Perchlorates. Chem. Mater. 2015, 27, 8126−8137. (33) The Five Classes of Fires and The Fire Extinguishers That Stop Them. http://www.strikeﬁrstusa.com/2016/05/ﬁve-classes-of-ﬁresﬁre-extinguishers-stop-them/ (Accessed 05−27-2019) (34) Category Archives: Formulas, Conversions & Calculations. https://web.archive.org/web/20120920075813/http://www. pelicanwire.com/category/formulas-resistance/ (Accessed 05−272019) (35) Magnetic susceptibility measurements of transition metal containing compounds. https://www.unf.edu/~michael.lufaso/chem3610L/ instructions_magnetic_susceptibility.pdf (Accessed 05−27-2019)